Abstract
The performance of a great variety of electronic devices—ranging from semiconductor transistors to superconducting qubits—is hampered by lowfrequency noise with spectra proportional to 1/f. The ubiquity and negative impact of 1/f noise has motivated intensive research into its cause, and it is now believed to originate from a bath of fluctuating twolevel defect states (TLSs) embedded in the material. This phenomenon is commonly described by the longestablished standard tunnelling model (STM) of independent TLS. A key prediction of STM is that the noise should vanish at low temperatures. Here we report measurements on superconducting microresonators over previously unattainable, very long time scales that show an increase in 1/f noise at low temperatures and low microwave power, contrary to the STM. We propose a new generalised tunnelling model that includes significant interaction between multiple TLSs, which fully describes these observations, as well as recent studies of individual TLS lifetimes in superconducting qubits.
Introduction
Initially introduced to explain unusual thermal properties of glasses with respect to crystals, the standard tunnelling model (STM)^{1,2} has enjoyed considerable success in describing many other phenomena in both ordered and disordered systems. The STM assumes the ability for a number of atoms at low temperatures to quantum mechanically tunnel between adjacent lattice sites. The model has since then been adopted to describe twolevel defect states (TLSs) in many other contexts: for example, TLS can be caused by tunnelling of electrons in insulating barriers, molecules with two quasistable configurations and so on^{3,4,5}. More generally, any influence of dilute impurities on macroscopic properties of materials is often parametrized as a bath of noninteracting TLSs, such that the STM is applicable. In particular, TLSs have been suggested as sources of the ubiquitous 1/f noise in electronic materials^{6} and are also active at low temperatures, where the kinetics is dominated by tunnelling^{7,8}. With the rapid recent progress of new devices for quantum information processing and detector applications, there is a renewed awareness^{9} of the deleterious effects of TLS noise. Here we demonstrate theoretically and experimentally that the STM fails in the extreme low temperature, lowpower limits where these new devices are typically operated; therefore, an extension of STM to include specific interactions between TLSs is necessary to address the shortcomings of this tried and trusted model.
The properties of TLSs can be conveniently studied using thinfilm highquality superconducting microwave resonators, which by themselves are important for a number of diverse applications ranging from quantum computation^{10} to submillimetre and farinfrared astronomy^{11}. Here TLSs, mainly located at interfaces, cause 1/f noise that manifests as an instability in the centre frequency. The mechanism can be understood by noting that TLSs behave as an ensemble of switching dipoles resulting in a fluctuating dielectric constant and induced electric noise in the resonator. Device performance can be severely hampered by the resulting jitter. Since a study of lowfrequency noise requires measurements that span a long time, the effects due to TLSs are often masked by unrelated instabilities in the resonator and the measurement system. There have been a number of studies of TLS noise in superconducting resonators^{12,13,14,15,16,17} to date; however, these results have not been explainable within the STM. This has motivated the development of new models that either assume the presence of additional sources of dissipation , for example, caused by edge defects^{18} or, alternatively, explain the shortcomings of the STM by reevaluating the underlying assumptions about the nature of TLS.
Here we demonstrate that the noise of superconducting microresonators^{19} increases as the temperature is decreased, an observation in direct contradiction to the STM. To account for these results we propose a new model, which includes significant interactions between TLSs. The interactions lead to spectral diffusion that alters the properties of the resonator. We show that besides explaining our results, the new model also explains results of other recent studies^{20} that used phase qubits as a way to probe individual TLS. We emphasize that these measurements were made possible through the use of an ultrastable Pound loop frequencytracking technique^{21} and specially designed lownoise epitaxial superconducting resonators with high temperature stability.
Results
Experimental results
We have performed a detailed study and analysis of the very lowfrequency noise in highquality Nb resonators. These measurements were performed in various microwave powers, down to average energies corresponding to ‹n›=1−10 photons in the resonator. A crucial feature of our measurements is the long measurement time (τ>10^{4 }s) leading to high statistical confidence. Two devices with different resonance frequencies, denoted Res1 and Res2, are studied in detail. The resonators (shown in Fig. 1a) are made of 50nmthick epitaxial Nb film with a 5nm Ptcapping layer grown by laser ablation on rplane sapphire (see Methods for details). The resonators have centre frequencies (ν_{0}) between 4–8 GHz, and intrinsic quality factors (Q) above 10^{5}. Further parameters can be found in Table 1 in the Methods section.
The measurements were performed by continuously monitoring the timevarying centre frequency ν_{0}(t). For all measurements presented in this work, the quantity of interest is the fractional frequency spectra (S_{y} in units of 1/Hz), which is defined by , where S_{dν} is the frequency spectra (in units of Hz^{2}/Hz), ν_{0} is the nominal centre frequency of the resonator and f(t_{i}) the Fourier frequency (see Methods for details).
The central result of this work is presented in Fig. 2, which shows the level of 1/f noise at 0.1 Hz plotted for the temperature range 60–500 mK at three different microwave drive levels; examples of full spectra can be found in Fig. 3a. For both resonators we find a stronger than 1/T temperature dependence for all microwave drives. These data can be fit to S_{y}(T)∝a/T^{1+μ}, where a is a powerdependent constant and μ=0.22±0.16 and μ=0.36±0.3 for Res1 and Res2, respectively. Hence, both sets of measurements suggest a temperature dependence stronger than 1/T. As will be shown later, μ turns out to be a microscopic parameter that can be directly related to the density of states of TLSs.
We also find that the 1/f noise level depends on the microwave drive or, more precisely, on the energy stored in the resonator, consistent with our previous results^{17}. At the highest powers (inset of Fig. 3b), we also see a saturation due to amplifier noise at a level consistent with other estimates^{18,22}. However, Fig. 3 shows that as power is decreased the resonator noise increases, until it saturates in the low power limit, at a level found to be temperaturedependent.
Examining possible noise mechanisms
We first discuss whether the jitter in the resonator frequency could be caused by inductance fluctuations from surface spins. The argument in favour of this is that inductance fluctuations according to ref. 23 exhibit a 1/f frequency dependence for T≲200 mK and that the noise level increases as the temperature is reduced in the range 100<T<2 K. However, it is to be noted that the details of the behaviour are very different to our observations: inductance noise acquires an approximate 1/f dependence only at the lowest temperatures, while at higher temperatures it is described by a much smaller exponent^{24}. Furthermore, at f~1 Hz the inductance noise is almost temperatureindependent and, crucially, for all frequencies the temperature dependence ceases below T≲200 mK. Finally, the power saturation of the noise seen in our resonators (Fig. 3b) implies that the frequency of the relevant excitation is close to the frequency of the resonator—for example, f~6 GHz. These frequencies are too large for a dilute spin system with the densities consistent with direct observations^{23,24}. To completely rule out spin as the dominant source of jitter, we performed measurements in weak (≈mT) inplane fields, which would be expected to affect these spin systems, but not the superconductor^{25}, and observe no change in the noise level.
Next, we consider whether the STM could describe the jitter in the resonator frequency. The central assumption of the STM is that certain atoms or groups of atoms may tunnel between two potential energy minima, which are separated in energy by an asymmetric splitting Δ_{0}. The tunnelling coupling energy is given by Δ~e^{−λ}, where λ is a tunnelling parameter proportional to the well separation and square root of the barrier height^{2}. The Hamiltonian of each TLS has the form , where σ^{i} (i=x, y, z) are the Pauli matrices. is the TLS energy splitting. The STM assumes that the energies Δ_{0} and Δ are uncorrelated and have joint probability distribution: in a wide (atomic) range of energies, with typical density of TLSs, which is materialdependent.
The TLSs interact with the external electric field and the strain field ε according to the Hamiltonian where is the electric dipole moment and γ is the elastic dipole moment. The effect of the interaction with the strain field can be seen as a renormalization of the asymmetry energy—that is, —therefore, it does not need to be treated separately. Different TLSs interact among themselves via long range dipole–dipole interaction (or phonon exchange) with an effective strength given by the dimensionless parameter with for electric (elastic) interactions. Here ? is the dielectric constant of the medium, ζ is the density of the glass and υ is the sound velocity. The dimensionless parameter is very small—that is, —such that within the STM interaction between TLS is assumed to be irrelevant. The dephasing and relaxation of the TLS is because of their interaction with phonons, giving a TLS relaxation rate , where k_{B} is the Boltzmann constant. The probability distribution of due to the distribution of Δ and Δ_{0} for a given E is wide and increases very rapidly near (ref. 26). Thermal fluctuations—absorption or emission of thermal phonons by an ensemble of independent TLSs—could cause a jitter in the resonator’s centre frequency (equivalent to a fluctuating dielectric constant Δε(r, t)). Since the number of activated TLSs is proportional to temperature and the effect of each TLS is small in T/ν_{0}, the STM predicts^{27} a noise spectrum that vanishes cubically for T<<hν_{0}/2k_{B}, in striking contrast to the results of Fig. 2. Moreover, in the regime of strong applied electric field our calculations show that one should expect a very weak power dependence of the noise spectra, in disagreement with the results of Fig. 3b. As such, the STM is completely incompatible with our results.
Other experimental studies have also found evidence for deviations from the STM. Individual TLS can be studied spectroscopically by superconducting qubits, allowing direct measurement of the relaxation time T_{1} and the dephasing time T_{2} of individual TLS^{28}. The temperature dependence of these lifetimes has also been studied^{20}, finding the expected wide distribution of relaxation rates for TLS, but in disagreement with STM predictions the temperature dependence of the relaxation rate is strong. Furthermore, the dephasing rate shows an anomalous behaviour: Γ_{2}~T^{1.24}. Studies of bulk ensembles of TLSs using highQ superconducting resonators have also found deviations from STM predictions with resonators showing a logarithmic power dependence in contrast to the square root dependence predicted by the STM^{29,30}. Second, the extracted density of states of TLS shows a weak power law dependence ρ(E)∝E^{μ}, with μ=0.28 (manuscript in preparation). This is in agreement with several studies in glasses where a slight suppression of the density of states at low energies ρ(E)∝E^{μ} with μ=0.3 was found^{31,32}. Finally, it was found that in thin oxide a−SiO_{2+x} layers, dipole–dipole interactions between TLSs may play a key role up to 100 mK^{33}.
All of this lead us to conclude that at least for thin oxide layers the STM does not correctly describe the properties of TLS.
The generalized tunnelling model
Our new model is conceptually shown in Fig. 1: a resonator (Fig. 1a) with centre frequency ν_{0} couples to an ensemble of coherent TLSs with energysplitting hν_{0}. Owing to nonnegligible interactions with surrounding TLS, the resonant TLS acquire a temperaturedependent width and are affected by strongly coupled slow incoherent (classical) fluctuators (Fig. 1b). The latter causes an energy drift bringing the resonant TLS in and out of resonance. One key prediction of this new model is that it results in a lowfrequency noise for a superconducting resonator that increases as the temperature is decreased. Moreover, this increase can be directly related to the microscopic parameter μ (introduced above), which is associated with the slight suppression of the density of TLS states at low energy. We argue that the noise observed in our measurements originates from thermally activated slow fluctuators that are also responsible for 1/f charge noise in superconducting devices^{34}. In particular, the resonator noise is generated by the switching of fluctuators that are located in the vicinity of quantum TLSs that are in resonance with the highfrequency electric field. In contrast to the STM, the interaction between TLSs is relevant for our model and the density of lowenergy states is slightly nonuniform. In fact, any significant interaction between local degrees of freedom leads to the suppression of density of states at low energies. The effect is most dramatic for longrange Coulomb interaction in three dimensions where it leads to the E^{2} dependence of the density of states known as the Efros–Shklovskii gap. Weaker but similar effect takes place for dipole–dipole interaction where similar arguments give a logarithmic energy suppression. It is not known whether higher orders of the perturbation theory give small power instead of the logarithm. It is also not excluded that experimental evidence for small power can be interpreted as a logarithmic correction. In this paper we adopt a phenomenological point of view that the density of states is described by a smallpower law^{35,36}. The assumption made in the STM that the size of the interaction is small is based on the hypothesis that the TLSs are local objects spaced at distances much larger than their size; however, this has never been proven experimentally—even for conventional glasses. (See Methods for details.)
We now show qualitatively that the assumptions of the dominant role of TLS–TLS interaction and the energydependent density of states explain the present data as well as the results of phase qubit experiments^{20,37}.
Similarly to that of optical homogeneous linewidth^{38}, the dephasing rate of the resonant TLS can be estimated by associating the dephasing process with the thermal relaxation of offresonant TLSs that interact strongly with it. Since for a density of states ρ(E)∝E^{μ}, the number of the offresonant TLSs is proportional to T^{1+μ}, the resulting width is Γ_{2}∝T^{1+μ}. Owing to this width, phononless relaxation processes between resonant TLSs become possible with rate Γ_{1}∝T^{1+μ}. Note that this power law is expected to hold at low temperature even while it dominates over the direct phonon emission. From our data we obtain μ≈0.2–0.4; as a result we get an estimate for the dephasing rate in very good agreement with the value μ=0.24 obtained from measurements of phase qubits. Furthermore, the wide distribution of relaxation rates implies the presence of very slow TLSs in the vicinity of the resonant ones. These very slow TLSs have coherence times much shorter than the tunnelling rate and thus they can be considered as classical fluctuators. Their presence is independently revealed by charge fluctuations that display a 1/f power spectrum^{34}. The effect of the classical fluctuators on the resonant quantum TLSs is to generate an energy drift of the TLS with a 1/f spectrum^{29}. However, this only occurs if the interaction strength between the classical and coherent TLS is greater than the TLS width—that is, if the slow fluctuators are located within a distance R_{max}=(U_{0}/Γ_{2})^{1/3} from the resonant quantum TLS. An important consequence of this picture is that the noise increases as the temperature decreases. This is because of the fact that as the width decreases with temperature the energy drift becomes more visible. As a result, with decreasing temperature the noise sensitivity increases, even if the number of thermally excited fluctuators decreases. Analytical computations based on Bloch equations^{39} give the following result for the noise spectrum:
where N_{f} is the number of strongly coupled fluctuators, is the Rabi frequency, is the applied electric field and V is the resonator volume. Using the measured value of μ≈0.36 (see Fig. 2) allows this equation to describe all the results reported in this work. We emphasize the agreement of this value with that usually obtained for various glasses.
Our model (see Methods) can also account for the power dependence (see Fig. 3b). In fact, since Γ_{1}Γ_{2}∝T^{2(1+μ)}, the saturation term becomes temperaturedependent. For low powers, the spectra have an overall strong temperature dependence proportional to T^{−(1+μ)}, whereas at high power our theory predicts that the temperature dependence of the spectra is constant. Figure 3b is a fit to the overall temperature and power dependence of the noise at 0.1 Hz: . In the fit, we used the measured value of μ≈0.36; where A and B are sampledependent parameters. We find that A≈4 × 10^{−16} for all temperatures. However, the value of B appears to change when the temperature is decreased below ~200 mK. For temperatures above 200 mK we find B=3.5 × 10^{−3} and for temperatures below 200 mK we find B=2.5 × 10^{−4}. As previously explained, the model is justified at lowest temperatures, so the observed crossover between the two regimes is not surprising. Although saturation is seen at all temperatures in Fig. 3, the saturation at the lowest temperature is the least clear. However, it should be noted that clear saturation in the low temperature limit has been observed elsewhere^{18}.
Discussion
The results of this work can be instructive in identifying the nature of TLS. The remarkable agreement between the noise data and our model of strongly interacting TLS seems to indicate that in thin oxide layers the assumption of pointlike defects needs to be revised. If TLSs are extended objects, the interactions between them can be significantly enhanced because they are effectively closer to each other and have a large dipole moment. The possibility of an extended nature of TLS was discussed, for example, in ref. 40. In addition, the observed rise of 1/f noise below ~1 K suggests that quantum devices, and in particular those comprising superconducting resonators, are not necessarily best operated at the lowest available temperatures. Instead, one should look for a sweet temperature spot with the largest signaltonoise ratio or the longest coherence time.
Finally, we note that the relevance of the interaction between TLSs in thin oxide layers does not contradict the existing body of data obtained previously on bulk amorphous materials. However, we do put forward the notion that results within literature on bulk materials may also benefit from a model including a dominant TLS–TLS interaction.
Methods
Samples
A 50nmthick epitaxial Nb film with a 5nm Ptcapping layer was grown by laser ablation on rplane sapphire substrate in an ultrahigh vacuum chamber with a base pressure of 10^{−9} Torr and at a growth temperature of 650 °C. The typical Nb films grown under these conditions^{41} were singlecrystalline Nb (100) with low surface roughness, 0.3–0.5 nm. The film was patterned into an array of resonators coupled to a common feedline on a 10 × 5 mm^{2} chip^{17,30} using optical lithography and dry etching in a 2:1 ratio SF_{6}/Ar plasma. The resonators used in our experiments are of the lumped element type, consisting of an inductive meander (inductance ~5 nH) in parallel with an interdigitated capacitor, see Fig. 1a. The centre frequency (ν_{0}) of these resonators is in the 4 to 8GHz band, and intrinsic quality factors (Q_{i}) above 10^{5}.
Measurements
A Pound frequency locked loop (described in detail in ref. 21) is used for all measurements. The high sensitivity and high bandwidth of this technique make it suitable for a variety of resonance measurements^{42,43} including noise measurements^{17}.
The intrinsic loss tangent—proportional to the concentration and dipole moment of TLS—of the resonators tan Δ_{i} was measured using the standard technique of fitting the ν_{0} versus T dependence^{30}. For both samples we find F tan Δ_{i}, where F is a filling factor of order 1, to be around 1 × 10^{−6} indicating very low dielectric loss.
Additional epitaxial samples without the Ptcapping layer were found to exhibit similar parameters but with Q_{i}≲100,000 and F tan Δ_{I}>2 × 10^{−6}, which is similar to previous work using sputtered Nb^{30}. The Ptcapping layer both increased Q_{i} by a factor of 5 and significantly reduced the dielectric loss tangent. This improvement is probably because of the Pt minimizing the intrinsic oxide layer on the niobium surface. As predicted by the STM theory, the presence of TLS gives rise to temperaturedependent resonant frequency shifts. However, the low loss tangent in our samples meant that a ±10mKtemperature fluctuation corresponds to a 200Hz frequency shift, which is smaller than the flicker noise level at −100dBm drive power^{17}. Such insensitivity to temperature fluctuations is a stringent requirement for measuring the temperature dependence of any slow process, which could otherwise be masked by temperatureinduced drifts.
All measurements were performed in a wellshielded dilution refrigerator equipped with a cryogenic HEMT amplifier and heavily attenuated microwave lines. Our measurement setup has been described elsewhere, see refs 17, 21.
Data analysis
The measured data were processed by calculating the overlapping Allan deviation (ADEV) from the acquired time series. Each ADEV was then prescreened for any signs of temperature drift, in which case the data set was discarded. By fitting to the 1/f part of the ADEV, which for these sample occur for t>0.01 s, we then parametrize the frequency noise as S_{y}∝h_{−1}/f, where S_{y} is the fractional frequency spectra, and extract h_{−1}. This is then used to plot the data in the more familiar form as the noise level at 0.1 Hz (calculated from the h_{−1} value).
Model
The measured noise in the resonator is because of the coupling between the TLS electric dipole moment and the applied electric field of the resonator. Our model assumes that:
(1) TLSs have the following probability distribution for the asymmetry energy Δ_{0} and the tunnelling energy Δ:
where
and values of μ are discussed in the text.
(2) TLS–TLS interactions are large and scale as 1/r^{3} (see below).
These two assumptions are in contrast to the STM^{1,2} where the asymmetry energy distribution is assumed to be constant and the interactions between TLSs are considered negligible. The large interaction between TLSs implies that a typical coherent TLS is strongly coupled to other coherent TLS. Here strongly coupled means that two TLSs have an interaction strength , where is the phononmediated relaxation rate for the TLS defined in the text. In this case, the mutual interaction results in an additional dephasing channel for the TLS. Calculations give a dephasing width Γ_{2}∝T^{1+μ} for TLS. In addition, strong interaction implies the presence of incoherent TLS (that is, classical fluctuators) strongly coupled to coherent TLS in resonance with the frequency of the resonator. Similarly to the coupling between coherent TLS, here strongly coupling means that U_{0}r^{−3}>Γ_{2}, so that slow fluctuators cause an energy drift for the resonant TLS: E(t)=E+ξ(t) with larger than the line width. Here N_{f} denotes the number of strongly coupled flucutators, r_{k} is the distance of the kfluctuator to the resonant TLS and n_{k}(t)=±1 is a random telegraph signal with associated switching rate γ_{k}. Note that these definitions of strong coupling imply that the scale of the interaction strength U_{0} might be still very small in absolute terms.
Additional information
How to cite this article: Burnett, J. et al. Evidence for interacting twolevel systems from the 1/f noise of a superconducting resonator. Nat. Commun. 5:4119 doi: 10.1038/ncomms5119 (2014).
References
 1.
Anderson, P. W., Halperin, B. & Varma, C. M. Anomalous lowtemperature thermal properties of glasses and spin glasses. Philos. Mag. 25, 1–9 (1972).
 2.
Phillips, W. Tunneling states in amorphous solids. J. Low Temp. Phys. 7, 351–360 (1972).
 3.
Rogers, C., Buhrman, R., Kroger, H. & Smith, L. Characterization of individual electron traps in amorphous si by telegraph noise spectroscopy. Appl. Phys. Lett. 49, 1107–1109 (1986).
 4.
Rella, C. et al. Vibrational echo studies of myoglobinCO. J. Phys. Chem. 100, 15620–15629 (1996).
 5.
Guimbretiere, G., Rufflé, B. & Vacher, R. Acoustic damping and dispersion in vitreous germanium oxide. Phys. Rev. B 86, 094304 (2012).
 6.
Black, R., Restle, P. & Weissman, M. Nearly traceless 1/f noise in bismuth. Phys. Rev. Lett. 51, 1476 (1983).
 7.
Ludviksson, A., Kree, R. & Schmid, A. Lowfrequency 1f fluctuations of resistivity in disordered metals. Phys. Rev. Lett. 52, 950–953 (1984).
 8.
Weissman, M. et al. 1/f noise and other slow, nonexponential kinetics in condensed matter. Rev. Mod. Phys. 60, 537–571 (1988).
 9.
Leggett, A. J. & Vural, D. C. “Tunneling twolevel systems” model of the lowtemperature properties of glasses: Are “smokinggun” tests possible? J. Phys. Chem. B 117, 12966–12971 (2013).
 10.
Wallraff, A. et al. Strong coupling of a single photon to a superconducting qubit using circuit quantum electrodynamics. Nature 431, 162–167 (2004).
 11.
Day, P. K., LeDuc, H. G., Mazin, B. A., Vayonakis, A. & Zmuidzinas, J. A broadband superconducting detector suitable for use in large arrays. Nature 425, 817–821 (2003).
 12.
Gao, J., Zmuidzinas, J., Mazin, B. A., LeDuc, H. G. & Day, P. K. Noise properties of superconducting coplanar waveguide microwave resonators. Appl. Phys. Lett. 90, 102507–102507 (2007).
 13.
Gao, J. et al. Experimental evidence for a surface distribution of twolevel systems in superconducting lithographed microwave resonators. Appl. Phys. Lett. 92, 152505–152505 (2008).
 14.
Kumar, S. et al. Temperature dependence of the frequency and noise of superconducting coplanar waveguide resonators. Appl. Phys. Lett. 92, 123503–123503 (2008).
 15.
Barends, R. et al. Noise in NbTiN, Al, and Ta superconducting resonators on silicon and sapphire substrates. IEEE Trans. Appl. Supercond. 19, 936–939 (2009).
 16.
Barends, R. et al. Minimal resonator loss for circuit quantum electrodynamics. Appl. Phys. Lett. 97, 023508–023508 (2010).
 17.
Burnett, J. et al. Slow noise processes in superconducting resonators. Phys. Rev. B 87, 140501 (2013).
 18.
Neill, C. et al. Fluctuations from edge defects in superconducting resonators. Appl. Phys. Lett. 103, 072601 (2013).
 19.
Zmuidzinas, J. Superconducting microresonators: physics and applications. Annu. Rev. Condens. Matter Phys. 3, 169–214 (2012).
 20.
Lisenfeld, J. et al. Measuring the temperature dependence of individual twolevel systems by direct coherent control. Phys. Rev. Lett. 105, 230504 (2010).
 21.
Lindstrom, T., Burnett, J., Oxborrow, M. & Tzalenchuk, A. Y. Poundlocking for characterization of superconducting microresonators. Rev. Sci. Instrum. 82, 104706–104706 (2011).
 22.
Murch, K., Weber, S., LevensonFalk, E., Vijay, R. & Siddiqi, I. 1/f noise of josephsonjunctionembedded microwave resonators at single photon energies and millikelvin temperatures. Appl. Phys. Lett. 100, 142601–142601 (2012).
 23.
Sendelbach, S., Hover, D., Mück, M. & McDermott, R. Complex inductance, excess noise, and surface magnetism in dc SQUIDs. Phys. Rev. Lett. 103, 117001 (2009).
 24.
Anton, S. et al. Magnetic flux noise in dc SQUIDs: Temperature and geometry dependence. Phys. Rev. Lett. 110, 147002 (2013).
 25.
Healey, J., Lindstrom, T., Colclough, M., Muirhead, C. & Tzalenchuk, A. Y. Magnetic field tuning of coplanar waveguide resonators. Appl. Phys. Lett. 93, 043513–043513 (2008).
 26.
Black, J. & Halperin, B. Spectral diffusion, phonon echoes, and saturation recovery in glasses at low temperatures. Phys. Rev. B 16, 2879 (1977).
 27.
Hunklinger, S., Arnold, W., Mason, W. P. & Thurston, R. Physical acoustics. Vol. XII (eds Mason W. P., Thurston R. N. p160Academic Press (1976).
 28.
Shalibo, Y. et al. Lifetime and coherence of twolevel defects in a Josephson junction. Phys. Rev. Lett. 105, 177001 (2010).
 29.
Faoro, L. & Ioffe, L. B. Internal loss of superconducting resonators induced by interacting twolevel systems. Phys. Rev. Lett. 109, 157005 (2012).
 30.
Lindström, T., Healey, J., Colclough, M., Muirhead, C. & Tzalenchuk, A. Y. Properties of superconducting planar resonators at millikelvin temperatures. Phys. Rev. B 80, 132501 (2009).
 31.
Zeller, R. & Pohl, R. Thermal conductivity and specific heat of noncrystalline solids. Phys. Rev. B 4, 2029 (1971).
 32.
Geva, E. & Skinner, J. Theory of singlemolecule optical lineshape distributions in lowtemperature glasses. J. Phys. Chem. B. 101, 8920–8932 (1997).
 33.
Ladieu, F., Le Cochec, J., Pari, P., Trouslard, P. & Ailloud, P. Dielectric constant of glasses: evidence for dipoledipole interactions. Phys. Rev. Lett. 90, 205501 (2003).
 34.
Kogan, S. Electronic Noise and Fluctuations in Solids Cambridge University Press (2008).
 35.
Efros, A. & Shklovskii, B. Coulomb gap and low temperature conductivity of disordered systems. J. Phys. C 8, L49 (1975).
 36.
Gorkov, L. & Eliashberg, G. Minute metallic particles in an electromagnetic field. Sov. Phys. JETP 21, 940 (1965).
 37.
Grabovskij, G. J., Peichl, T., Lisenfeld, J., Weiss, G. & Ustinov, A. V. Strain tuning of individual atomic tunneling systems detected by a superconducting qubit. Science 338, 232–234 (2012).
 38.
Lyo, S. Anomalous optical homogeneous linewidths in glasses. Phys. Rev. Lett. 48, 688 (1982).
 39.
Bloch, F. Generalized theory of relaxation. Phys. Rev. 105, 1206 (1957).
 40.
Lubchenko, V. & Wolynes, P. G. Intrinsic quantum excitations of low temperature glasses. Phys. Rev. Lett. 87, 195901 (2001).
 41.
Mikhailov, G., Malikov, I., Chernykh, A. & Petrashov, V. The effect of growth temperature on electrical conductivity and on the structure of thin refractory metal films, grown by laser ablation deposition. Thin Solid Films 293, 315–319 (1997).
 42.
de Graaf, S. E. et al. Charge qubit coupled to an intense microwave electromagnetic field in a superconducting Nb device: Evidence for photonassisted quasiparticle tunnelling. Phys. Rev. Lett. 111, 137002 (2013).
 43.
de Graaf, S. E., Danilov, A., Adamyan, A. & Kubatkin, S. A nearfield scanning microwave microscope based on a superconducting resonator for low power measurements. Rev. Sci. Instrum. 84, 023706–023706 (2013).
Acknowledgements
We thank M. Kataoka for critical reading of the manuscript, and M. Gustafsson, S. de Graaf, L. Ioffe, S. Anton and J. Clarke for fruitful discussions. This work was supported by NMS, the EPSRC and by ARO W911NF1310431.
Author information
Affiliations
National Physical Laboratory, Hampton Road, Teddington TW11 0LW, UK
 J. Burnett
 , I. Wisby
 , A. Ya. Tzalenchuk
 & T. Lindström
Royal Holloway, University of London, Egham TW20 0EX, UK
 J. Burnett
 , I. Wisby
 , R. Shaikhaidarov
 , V. Antonov
 , P. J. Meeson
 & A. Ya. Tzalenchuk
Laboratoire de Physique Theorique et Hautes Energies, CNRS UMR 7589, Universites Paris 6 et 7, 4 place Jussieu, Paris 75252, Cedex 05, France
 L. Faoro
Department of Physics and Astronomy, Rutgers The State University of New Jersey, 136 Frelinghuysen Road, Piscataway, New Jersey 08854, USA
 L. Faoro
Institute of Microelectronics Technology and High Purity Materials, Academician Ossipyan strasse, 6, Chernogolovka, Moscow 142432, Russia
 V. L. Gurtovoi
 , A. V. Chernykh
 , G. M. Mikhailov
 & V. A. Tulin
Authors
Search for J. Burnett in:
Search for L. Faoro in:
Search for I. Wisby in:
Search for V. L. Gurtovoi in:
Search for A. V. Chernykh in:
Search for G. M. Mikhailov in:
Search for V. A. Tulin in:
Search for R. Shaikhaidarov in:
Search for V. Antonov in:
Search for P. J. Meeson in:
Search for A. Ya. Tzalenchuk in:
Search for T. Lindström in:
Contributions
J.B., T.L., A.Y.T. planned the experiment, T.L. designed the samples, V.A. came up with the idea of epitaxial films with conducting coating. A.V.C., G.M.M.,V.L.G.,V.A.T. produced the films, R.S. and V.A. patterned the devices. J.B., I.W. and T.L. performed the measurements, J.B., T.L. and L.F. performed the data analysis, L.F. developed the theory and discussed the results. P.J.M. contributed to the discussion and provided support, J.B., L.F., T.L., A.Y.T. wrote the manuscript with feedback from all authors including significant contributions from I.W., V.A. and V.L.G.
Competing interests
The authors declare no competing financial interests.
Corresponding author
Correspondence to T. Lindström.
Rights and permissions
To obtain permission to reuse content from this article visit RightsLink.
About this article
Further reading

Suppression of lowfrequency charge noise in superconducting resonators by surface spin desorption
Nature Communications (2018)

Observation and coherent control of interfaceinduced electronic resonances in a fieldeffect transistor
Nature Materials (2017)

Observation of directly interacting coherent twolevel systems in an amorphous material
Nature Communications (2015)

Coherent interaction with twolevel fluctuators using near field scanning microwave microscopy
Scientific Reports (2015)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.